APS sprayed coatings onto the selective laser melted substrates
APS sprayed coatings onto
the selective laser melted substrates
Powłoki aPs natryskiwane na podłoża przetapiane wiązką laserową abstract
Additive layer-based selective laser melting technologies (SLm), provide a new range of possibilities for objects manufacturing. In the present study the alumina/
titania Al2O3/TiO2 coatings were applied onto SLm-manufactured substrates by the atmospheric plasma spraying method. The microstructure and porosity of coatings
were examined by scanning electron microscopy (SEm),
and industrial computer tomography. Bonding strength of
the coatings was analysed.
Selective laser melting SLm is an additive manufacturing process based on the layered forming of physical
objects by fusing of materials in the form of powder.
This method allows processing for wide range of metal powders including stainless steels, tool steels, as
well as Cr-Co and Ti alloys. The SLm technology is the
process of total metal powders melting using the controlled beam of 100 W (up to 400 W), 1064 nm wave
length, nd:YAG fibre laser [1, 2]. The process of melting
runs in the protective atmosphere of argon preventing
against oxidation of the fused metal powders. Due to
the layered incremental process of manufacturing and
the wide range of available materials the technology
could be applied for creating physical objects of complex geometrical structure both, internal and external.
The SLm process finds application in manufacturing
prototypes, final products , as well as tools, involving
inserts of injection moulds  or stamping die parts.
Dr inż. Mariusz Frankiewicz, prof dr hab. inż. Edward Chlebus, mgr inż. Karol Kobiela – Politechnika Wrocławska.
Generatywne technologie selektywnego przetapiania
laserowego (SLm) zapewniają nowe możliwości wytwarzania części maszyn. W pracy badaniom poddano powłoki tlenku glinu i tytanu Al2O3/TiO2 nanoszone za pomocą metody natryskiwania plazmowego APS na podłoża
wykonane w procesie SLm. Przy zastosowaniu skaningowej mikroskopii elektronowej i przemysłowej tomografii komputerowej przeprowadzono ocenę mikrostruktury
i porowatości powłok, jak również poddano analizie przyczepność powłok.
Operating properties of objects manufactured using
the selective laser melting method may be improved by
applying additional surface engineering treatment such
as the functional coating deposition.
One of the methods of improving properties of components manufactured in the SLm process is plasma
spraying. In the plasma spraying processes the material in a form of powder is supplied to plasma gun
(plasmatron), fused and then deposited onto a substrate surface with a velocity of approximately 150 m/s.
Functional coatings deposited with this method may
be, among others, characterised with: resistance to diffusion, low friction coefficient, resistance to low- and
high-temperature corrosion in aggressive chemical
environment, as well as high surface hardness and
high wear resistance [4, 5].
The plasma-sprayed Al2O3/TiO2 coatings provide
a high wear resistance properties, are applied among
others, in the textile, machinebuilding and paper industries [6÷8]. Alumina/titania coatings are known to be
dense, with smooth as-sprayed surface. Alumina/titania with 3% share by weight of TiO2 (97/3) has been
applied for preventing wear, as well as chemical and
cavitational erosion in pump components . Also,
the variation of Al2O3/TiO2 composition with increased
Przegląd sPawalnictwa 9/2012
to 13% share by weight of TiO2 is used (Al2O3 – 13%,
TiO2). Increase in share of titanium dioxide improves
the crack resistance . For tests the material supplied
by BayState Surface Tech designated as PP-37 (Al2O3
– 3%, TiO2) was used.
The research were aimed at initial analysis of coatings deposited by plasma spraying at substrates manufactured by the selective laser melting process. For
that purpose the tests of surface profile, using confocal
microscopy, industrial computer tomography and SEm
were applied. The tests were performed with the purpose of evaluating the influence of substrate surface
characteristics at the coating adhesion degree.
Fig.2.Profilogram of the unmachined sample surface
Rys.2. Profil nieobrobionej powierzchni próbki
The substrates were made of the Ti6Al7nb titanium
alloy  by the SLm Realizer II system. Orientation
of the analysed substrate surface during SLm manufacturing process has been presented in Fig. 1. The
research was carried out on four sets of five samples
each. Three sets were grit-blasted with three different
energies of abrasive material stream each (Al2O3 with
grain size of 120 µm), related to the three values of aluminium oxide feeding pressure, presented in the Table
I. One set of the samples was coated without additional
machining of the substrate surface.
The first stage of the research was aimed on identification of the influence of the grit-blasting parameters
Fig.1.View of the analysed surface of the SLm manufactured sample
Rys.1. Analizowana powierzania próbki wytwarzanej metodą SLm
tableI.Results of the substrate average roughness analyses before
tablicaI.Wyniki analizy średnich wartości chropowatości przed nałożeniem powłoki
Type of sample surface
Grit blasted surface, set no. 1
Grit blasted surface, set no. 2
Grit blasted surface, set no. 3
Przegląd sPawalnictwa 9/2012
Fig.3.Profilogram of the grit-blasted sample surface. Feeding pressure of 0,6 mPa
Rys.3.Profil obrobionej strumieniowo powierzchni próbki. Ciśnienie
wejściowe 0,6 mPa
on the geometrical structure of the substrate. Roughness analysis of the surfaces was performed using the
Rank Taylor Hobson Form Talysurf 1201 profilographometer. Example results of the measurements for nonmachined surfaces have been presented in Fig. 2, and
for the grit-blasted ones in Fig. 3.
In addition, an analysis of surface roughness was
performed using the LEXT OLS4000 confocal microscope.
Results of the analyses of substrate surface not
subjected to grit-blasting processing have shown that
they are characterised with a structure containing
non-melted powder grains. They adhere to the melted surfaces of the samples during the selective laser
melting process. Character of the non-machined SLm
surface may be observed in Fig. 4. Diameters values of the non-melted grains, ranging from several to
about 70 µm, lead to high surface roughness of the
SLm manufactured objects. Results of the roughness
measurements carried out on the grit-blasted surfaces shows decreasing values of the Ra parameter, on
average from above 15,25 µm up to about 8,58 µm,
as shown in Fig. 3. Character of the Ra changes can
be explained as a result of removal of the non-melted
powder grains partly agglomerated with the surface.
Increasing of roughness for the third set of samples,
tableII.Parameters of plasma burner operation during test coatings
tablicaII.Parametry procesu podczas natryskiwania powłok próbnych
Fig. 4. View of the substrate surface as observed in the confocal
Rys.4.Powierzchnia podłoża obserwowana na mikroskopie współogniskowym
Ar flow, l/min
He flow, l/min
Fig.6.Example of CT image of the coating (top) and substrate (bottom) porosity. Coating deposited on the grit-blasted substrate
Rys.6. Przykład obrazu CT porowatości powłoki (u góry) i podłoża
(u dołu). Powłoka naniesiona na obrobione strumieniowo podłoże
Fig.7. View of spatial qualitative analysis of arrangement
and morphology of the coating
Rys. 7. Jakościowa analiza
przestrzenna rozmieszczenia i
morfologii nieciągłości powłoki
Fig.5. View of the substrate surface after grit-blasting with 0,5 mPa
Rys.5.Powierzchnia podłoża obrobiona strumieniowo przy ciśnieniu
wejściowym 0,5 mPa
which was processed with 0,6 mPa feeding pressure,
can be linked to the higher energy of the abrasive material stream and should be investigated in the further
research. microscopic view of the grit-blasted surface
has been presented in Fig. 5.
Results of the surface roughness analyses have
been collected in Table I.
Coatings were sprayed by the APS 60 kW robotised plasma spraying system equipped with the BayState Surface Tech SG100 plasma burner. Sample
coatings were deposited with parameters presented
in Table II.
The second stage of investigations was analyses
of the internal structure with the using of the industrial tomography method (CT). It was carried out by
the Zeiss metrotom CT equipment with a detector of
1024x1024 pixels resolution and the 225 kV lamp enabling achievement of 10 µm measurements resolution.
The CT tests enabled determining porosity of the deposited coatings. Exemplary result of porosity analysis
for coating deposited on the grit-blasted surface, has
been presented in Fig. 6. It was characterised with banding location of the pores resulting from the coating deposition process. Subsequent layers of the deposited
Fig.8.Example of SEm images of the coating (top) and substrate
(bottom) cross-section: a) overall view with coating thickness marked, b) detailed view of the coating pores. Coating deposited at the
Rys.8.Przykładowe obrazy SEm przekroju powłoki (u góry) i podłoża (u dołu): a) widok całej grubości powłoki, b) powiększenie obszaru z porowatością powłoki. Powłoka nanoszona na nieobrobione
Przegląd sPawalnictwa 9/2012
Fig.9.SEm image of defects in the Al2O3/TiO2 coating resulting from
complex structure of the substrate surface. Coating deposited at the
Fig.9. Obraz SEm wad w powłoce Al2O3/TiO2 wynikających ze złożonej struktury podłoża. Powłoka nanoszona na nieobrobione podłoże
Fig.10. Example SEm image of coating (top) deposited at grit-blasted substrate (bottom)
Rys. 10. Przykładowy obraz SEm powłoki (u góry) nanoszonej na
obrobione podłoże (u dołu)
coating were separated by bands of pores. Fig. 6 presents
the pore bands located in 4 layers between 5 deposited
layers of the coating. It was not observed pores on the
layer between the substrate and the coating, which allowed assumption on its high adherence to the substrate.
The results of porosity analysis for coatings deposited
on the non-machined substrates, showed discontinuity
of the coating on the layer between coating and substrate.
Also, porosity of the coated substrate has been
observed, as seen in Fig. 6, that is characteristic for
substrates manufactured with the SLm method. Size
and arrangement of the pores could be parameters, the
values of which are controlled by selecting the proper
parameters for the selective laser melting process, involving, among others, the laser power and scanning
rate of the layer fused with a laser beam .
CT analysis results have been verified by SEm
tests, performed at transverse microsections of the
samples with deposited coatings. measurements
of coating thicknesses were performed at them, which
have shown similar values amounting to about 450 µm.
The coating structure discontinuities observed during CT analysis, corresponded to its defects found
during analysis using SEm, see Fig. 8 and Fig. 9. Their presence could be related to the complex geometrical surfaces structure of substrates manufactured
with the SLm. The non-melted Ti6Al7nb powder grains agglomerated to its surface could prevent correct
deposition of coating at the whole substrate surface,
which is visible in Fig. 9. In the SEm images of the
cross-sections of coating samples deposited at gritblasted substrates much lower number of coating defects was observed at the junction with the substrate
surface, see Fig. 10. The observed regularity results
from removal of the Ti6Al7nb powder grains weakly
bound with the substrate by means of grit-blasting,
which resulted in better adhesion of the coating, as
seen on Fig. 10.
 Chlebus E., Kuźnicka B., Kurzynowski T., Dybała B.: microstructure and mechanical behaviour of Ti-6Al-7nb alloy produced by selective laser melting, materials Characterization 62,
2011, s. 488-495.
 Chlebus E.: Rapid prototyping and advanced manufacturing.
Springer handbook of mechanical engineering / [Karl-Heinrich] Grote, [Erik K.] Antonsson (eds.). Berlin: Springer, 2009,
 Frankiewicz m., Kurzynowski T., Dybała B., Chlebus E.: Rapid
Tooling application in manufacturing of injection moulds, Virtual design and automation/ed. by Z. Weiss. Poznań : Publishing
House of Poznan University of Technology, 2008. s. 155-162.
 Heinmann R.: Plasma Spray Coating, John Wiley & Sons, Ltd,
Chichester, UK, 2008.
 Pawlowski L.: The Science and Engineering of Thermal Spray
Coatings, John Wiley & Sons, Ltd, Chichester, UK, 2008.
Przegląd sPawalnictwa 9/2012
 Rico A., Poza P., Rodríguez J.: High temperature tribological
behavior of nanostructured and conventional plasma sprayed
alumina-titania coatings, Vacuum, Available online 2 march
2012, ISSn 0042-207X.
 Venkataraman R., Gautam Das a, Venkataraman B., narashima Rao G.V., Krishnamurthy R.: Image processing and statistical analysis of microstructures of as plasma sprayed Alumina-13 wt.% Titania coatings, Surface & Coatings Technology
201, 2006, s. 3691-3700.
 Yugeswaran S., Selvarajan V., Vijay m., Ananthapadmanabhan P.V., SreekumarK.P.: Influence of critical plasma spraying parameter (CPSP) on plasma sprayed Alumina–Titania
composite coatings, Ceramics International 36, 2010, s. 141149.